Presentation on theme: "Fundamental of Metal Casting"— Presentation transcript:
1Fundamental of Metal Casting Manufacturing Processes, 1311Dr Simin NasseriSouthern Polytechnic State University
2FUNDAMENTALS OF METAL CASTING Overview of Casting TechnologyHeating and PouringSolidification and Cooling
3Solidification Processes Starting work material is either a liquid or is in a highly plastic condition, and a part is created through solidification of the materialSolidification processes can be classified according to engineering material processed:MetalsCeramics, specifically glassesPolymers and polymer matrix composites (PMCs)
4Figure 10.1 Classification of solidification processes.
5CastingProcess in which molten metal flows by gravity or other force into a mold where it solidifies in the shape of the mold cavityThe term casting also applies to the part made in the processSteps in casting seem simple:Melt the metalPour it into a moldLet it freeze
6Capabilities and Advantages of Casting Can create complex part geometriesCan create both external and internal shapesSome casting processes are net shape; others are near net shapeCan produce very large parts (even 100 tons!)Can be performed on any metal that can be heated to the liquid stateSome casting methods are suited to mass production
7Disadvantages of Casting Limitations on mechanical propertiesPoor dimensional accuracy and surface finish for some processes; e.g., sand castingSafety hazards to workers due to hot molten metalsEnvironmental problems
8Parts Made by CastingAll varieties of metals can be cast, ferrous and nonferrousBig partsEngine blocks and heads for automotive vehicles, wood burning stoves, machine frames, railway wheels, pipes, church bells, big statues, pump housingsSmall partsDental crowns, jewelry, small statues, frying pans
9Overview of Casting Technology Casting is usually performed in a foundryFoundry = factory equipped for making molds, melting and handling molten metal, performing the casting process, and cleaning the finished castingWorkers who perform casting are called foundrymen
10The Mold in CastingContains cavity whose geometry determines part shapeActual size and shape of cavity must be slightly oversized to allow for shrinkage of metal during solidification and coolingMolds are made of a variety of materials, including sand, plaster, ceramic, and metal
11Open Molds and Closed Molds Figure Two forms of mold: (a) open mold, simply a container in the shape of the desired part; and (b) closed mold, in which the mold geometry is more complex and requires a gating system (passageway) leading into the cavity.
12Two Categories of Casting Processes Expendable mold processes – uses an expendable mold which must be destroyed to remove castingMold materials: sand, plaster, and similar materials, plus bindersExample: Sand castingPermanent mold processes – uses a permanent mold which can be used over and over to produce many castingsMade of metal (or, less commonly, a ceramic refractory material)Example: Die casting
13Advantages and Disadvantages Expendablemold processPermanentmold processPart shapes in permanent mold processes are limited by the need to open the mold.Permanent mold processes are more economic in high production operations.After the metal hardens, the mold must be scarified in order to recover the casting.More complicated geometries are possible with expendable mold processes.
14Sand Casting Mold Mold consists of two halves: Cope = upper half of moldDrag = bottom halfMold halves are contained in a box, called a flaskThe two halves separate at the parting lineFigure 10.2 (b) Sand casting mold.
15Forming the Mold Cavity Mold cavity is formed by packing sand around a pattern, which has the shape of the partWhen the pattern is removed, the remaining cavity of the packed sand has desired shape of cast partThe pattern is usually oversized to allow for shrinkage of metal during solidification and coolingSand for the mold is moist and contains a binder to maintain its shape
16Forming the Mold Cavity http://www. metalwebnews One half of the pattern is placed at the bottom.Open the mold and remove the pattern before pouring the metal
17Use of a Core in the Mold Cavity The mold cavity provides the external surfaces of the cast partIn addition, a casting may have internal surfaces, determined by a core, placed inside the mold cavity to define the interior geometry of partIn sand casting, cores are generally made of sand
18Gating System and Riser At the top of downsprue, a pouring cup is often used to minimize splash and turbulence as the metal flows into downsprueChannel through which molten metal flows into cavity from outside of mold consists of a downsprue, through which metal enters a runner leading to the main cavityRiser is a reservoir in the mold which is a source of liquid metal to compensate for shrinkage of the part during solidification
19Heating the Metal Heat to raise temperature to melting point Heating furnaces are used to heat the metal to molten temperature sufficient for castingThe heat required is the sum of:Heat to raise temperature to melting pointHeat of fusion to convert from solid to liquidHeat to raise molten metal to desired temperature for pouring
20Pouring the Molten Metal For this step to be successful, metal must flow into all regions of the mold, most importantly the main cavity, before solidifyingFactors that determine successPouring temperaturePouring rateTurbulence
21Solidification of Metals Transformation of molten metal back into solid stateSolidification differs depending on whether the metal isA pure element orAn alloy
22Cooling Curve for a Pure Metal A pure metal solidifies at a constant temperature equal to its freezing point (same as melting point)Figure Cooling curve for a pure metal during casting.
23Solidification of Pure Metals Due to chilling action of mold wall, a thin skin of solid metal is formed at the interface immediately after pouringSkin thickness increases to form a shell around the molten metal as solidification progressesRate of freezing depends on heat transfer into mold, as well as thermal properties of the metalFigure Characteristic grain structure in a casting of a pure metal, showing randomly oriented grains of small size near the mold wall, and large columnar grains oriented toward the center of the casting.
24Solidification of Alloys Most alloys freeze over a temperature range rather than at a single temperatureFigure (a) Phase diagram for a copper‑nickel alloy system and (b) associated cooling curve for a 50%Ni‑50%Cu composition during casting.
25Solidification of Alloys Figure Characteristic grain structure in an alloy casting, showing segregation of alloying components in center of casting.
26Solidification Time Solidification takes time Total solidification time TTS = time required for casting to solidify after pouringTTS depends on size and shape of casting by relationship known as Chvorinov's Rulewhere TST = total solidification time;V = volume of the casting;A = surface area of casting;n = exponent with typical value = 2; andCm is mold constant.
27Mold Constant in Chvorinov's Rule Mold constant Cm depends on:Mold materialThermal properties of casting metalPouring temperature relative to melting pointValue of Cm for a given casting operation can be based on experimental data from previous operations carried out using same mold material, metal, and pouring temperature, even though the shape of the part may be quite different
28What Chvorinov's Rule Tells Us A casting with a higher volume‑to‑surface area ratio cools and solidifies more slowly than one with a lower ratioTo feed molten metal to main cavity, TST for riser must be greater than TST for main casting (molten metal solidifies in riser after the molten metal is solidified in the main casting)How do they control this?!!Since mold constants of riser and casting will be equal, design the riser to have a larger volume‑to‑area ratio so that the main casting solidifies firstThis minimizes the effects of shrinkage
29Solidification Shrinkage Occurs in nearly all metals because the solid phase has a higher density than the liquid phaseThus, solidification causes a reduction in volume per unit weight of metalException: Do you know any metal which expands during solidification?!Cast iron with high C contentGraphitization during final stages of freezing causes expansion that counteracts volumetric decrease associated with phase change
30Shrinkage in Solidification and Cooling Figure Shrinkage of a cylindrical casting during solidification and cooling: (0) starting level of molten metal immediately after pouring; (1) reduction in level caused by liquid contraction during cooling (dimensional reductions are exaggerated for clarity).
31Shrinkage in Solidification and Cooling Figure (2) reduction in height and formation of shrinkage cavity caused by solidification shrinkage; (3) further reduction in height and diameter due to thermal contraction during cooling of solid metal (dimensional reductions are exaggerated for clarity).
32Shrinkage AllowancePatternmakers account for solidification shrinkage and thermal contraction by making mold cavity oversizedAmount by which mold is made larger relative to final casting size is called pattern shrinkage allowance
33Directional Solidification To minimize damaging effects of shrinkage, it is desirable for regions of the casting most distant from the liquid metal supply to freeze first and for solidification to progress from these remote regions toward the riser(s)Thus, molten metal is continually available from risers to prevent shrinkage voidsThe term directional solidification describes this aspect of freezing and methods by which it is controlled
34Achieving Directional Solidification Desired directional solidification is achieved using Chvorinov's Rule to design the casting itself, its orientation in the mold, and the riser system that feeds itLocate sections of the casting with lower V/A ratios away from riser, so freezing occurs first in these regions, and the liquid metal supply for the rest of the casting remains open
35External ChillsChills ‑ internal or external heat sinks that cause rapid freezing in certain regions of the castingFigure (a) External chill to encourage rapid freezing of the molten metal in a thin section of the casting; and (b) the likely result if the external chill were not used.
36Riser DesignRiser is waste metal that is separated from the casting and remelted to make more castingsTo minimize waste in the unit operation, it is desirable for the volume of metal in the riser to be a minimumSince the geometry of the riser is normally selected to maximize the V/A ratio, this allows riser volume to be reduced to the minimum possible value